1.
International Journal of Engineering Research and DevelopmentISSN: 2278-067X, Volume 1, Issue 2 (May 2012), PP.34-39www.ijerd.com F.E. Analysis and Experimental Investigation of Effect of Reinforcement Dimensions on Vibration Characteristics of Polypropylene Composite Satnam Singh1, N.K. Batra2, Rekha Rattan3 1, 2, 3 Department of Mechanical Engineering, Maharishi Markandeshwar University, Mullana, IndiaAbstract––Composites are being used everywhere nowadays. Their increased utilization necessitates their detailed studybefore putting them in actual use. Vibration characteristics are one of the important parameters which have to be studiedfor safe utilization of composites in various field specially related to antivibration applications. Damping behaviordirectly relates materials ability to absorb shocks and vibrations without getting damaged. Phase Lag gives the measureof damping capacity of any material. Reinforcement types also contribute towards damping behavior. In present workdamping behavior of unreinforced material, long glass fiber reinforced and short glass fiber reinforced polypropylenematerial are examined experimentally. Effect of reinforced fibers dimensions are first studied numerically using F.E.software Ansys. Results of F.E. analysis will provide composite with greater interfacial strength. Increased interfacialstrength increases the ability of material to absorb shocks and vibrations without getting fractured, thus absorbing moreenergy and providing increased damping capacity. Experimental results confirms that presence of reinforced fibersincreases the damping capacity and among reinforcements, short fiber reinforced polypropylene shows increaseddamping capacity then long glass fiber reinforced.Keywords––polymer composite, polypropylene, reinforcement, F.E. analysis, damping behavior I. INTRODUCTION High damping capacity materials allows undesirable mechanical vibrations and wave propagation to suppress.Polymer composite materials are being used for many antivibration applications due to their excellent properties ofdamping behavior, resilience and creep resistance. Especially due to its high specific strength to weight and stiffness toweight ratios composite materials are finding many aerospace applications [1]. Presence of discontinuous fibers makes ittheoretically possible to improve damping behavior of composite [2-3]. C. Subramanian [4] invested the effect ofreinforced fiber length on the leaf spring performance under dynamic load conditions and confirmed that long fibers cancarry three times more load then short fiber composite but the damping behavior of short glass fiber reinforced leaf springis found to be superior to that of long glass fiber reinforced leaf spring. Rakesh Chandra et al. [5] predicted the dampingin three-phase fiber-reinforced composites using finite element analysis and concluded that by optimizing theproperties/parameters of interphase (i.e., moduli, loss factors/size and physical state) appropriate level of damping can beachieved in fiber-reinforced composites under different conditions. R.F. Gibson et al. [6] studied the effects of the size ofthe fiber-matrix interphase on composite damping and described the use of a general purpose strain energy/finite elementmethod for micromechanical modeling of both damping and stiffness in composites. E. J. Lavernia et al. [7] studied thedamping behavior of metal matrix composites with discontinuous reinforcements. Experimental damping measurementswere carried out on short fiber and long fiber reinforced composites and concluded that short fiber composites showsmore damping and increased natural frequency by Amit Kumar Haldar et al. [8]. Excessive vibrations may generate highnoise levels, stress fatigue failure, premature wear, and unsafe operating conditions. To avoid these potential problems,there is a need to understand the complete vibration response of these materials. A new simulation model was proposedthrough measuring the damping factor of fiber reinforced thermoplastic parts and the experimental model analysis of theparts [9]. Hassan et al. [10] investigated the properties of injection molded short and long carbon fiber reinforcedpolyamide material. Fiber length characteristics were found to be in agreement with the improved tensile strength andtensile modulus of long fiber composites over the short fiber composites, despite the reduction in their fracture strain. Leeet al. [11] conducted flexural and torsional vibration tests to obtain dynamic characteristics of carbon fiber reinforcedPEEK. Measured natural frequency and specific damping capacity were compared with finite element results and foundto be in good agreement. Present work aims at the finite element analysis of long fiber and short multi fiber to predict theinterfacial strength. Composite with high interfacial strength or less interfacial stress will show higher damping capacity,which will be verified experimentally. II. FINITE ELEMENT MODELING OF LONG SINGLE AND SHORT MULTI FIBER MODEL AND ANALYSIS The FEA method is used to model composite material on the micro-mechanical level. Consider a fiber–matrixspecimen, whose geometry is shown in Fig. 1. The commercial FE software ANSYS is used in the FE simulation. Due toaxisymmetry, the specimen can be considered as a 2-D elastic body and 4-node quadrilateral element PLANE42 is usedin the analysis. 34
2.
F.E. Analysis and Experimental Investigation of Effect of Reinforcement DimensionsFollowing parameters are used in analysis [12]:1). Fibers are glass fibers with Young’s modulus Ef =75 GPa, and Poisson ratio Vf = 0.22). Matrix is of polypropylene with Young’s modulus Em=1.05 GPa and Poisson ratio Vm=0.33.Following two cases are considered for F.E. analysis:1). Tensile interfacial stress distribution along length interface at 20% and 40% volume fraction of single long fiber embedded in matrix as shown in figure 1.2). Tensile interfacial stress distribution along length interface of short multi fiber model such that volume fraction offibers remain same as that of single fiber. This model allows to study the effect of fiber dimensions on stress distribution.FEA models of fiber embedded in matrix are shown in figure 1. which are considered to understand the micromechanicalbehavior of composite. This unit cell domain geometry is defined in terms of the following parameters: : Length, diameter and radius of the fiber : Length, diameter and radius of the matrix.Fiber aspect ratio:Fiber spacing parameter:The dimensions of the unit cell are hence related to the volume fraction of the fibers in the composite by equation (1)[13]: (Eq. 1)Where = volume fraction of fibers in matrix Disp Disp . Matrix . Dm Dm Lm Df Df Lf Vy=0 Vy=0 Fibers Figure 1: Single long fiber and double short fiber models 35
3.
F.E. Analysis and Experimental Investigation of Effect of Reinforcement DimensionsTable 1 show the dimensions of models at 20% and 40% of volume fraction of fibers, at fixed aspect ratio of 20, whichare obtained by using equation 1. Type of Composite Volume Fraction Matrix Dimensions (µm) Fiber Dimensions (µm) Lm Dm Lf Df Long Single Fiber Model 20% 150 7.5 87.72 4.38 40% 150 7.5 110.52 5.52 Short Double Fiber 20% 150 7.5 69.62 3.48 Model 40% 150 7.5 87.72 4.38 Table 1: Dimensions of long single fiber and short double fiber model for 20% and 40% volume fraction2.1 Boundary Conditions Both composites at same volume fractions are subjected to same boundary conditions of Vy = 0 i.e. models havezero displacement in y direction and constant displacement of 1.8 µm is applied on the top of models at Y=L m. F.Eanalysis results are shown in fig. 5 and fig. 6. III. TEST MATERIAL FOR VIBRATION ANALYSIS Unreinforced, long glass fiber and short glass fiber reinforced polypropylene materials were hand molded andsubjected to forced vibration to understand the vibration and damping behavior of thermoplastic composites. Testmaterials were molded into rectangular specimen of size (120 X 12 X 3 mm) as shown in figure 2. Fiber volume was20% of total volume of composite for both long and short fibers. Figure 2: Test specimen3.1 Experimental Setup for Forced Vibrations Experimental arrangement for the forced transverse vibrations of the composite specimen is shown in fig.3.Specimen is clamped at one end on a mounting and the force transducer is fixed above the exciter and connected to thecantilever beam. An accelerometer is fixed above the cantilever beam at free end and the signal from the accelerometerand force transducer is fed to the data acquisition and the FFT analysis was made. The power supply is given to theexciter through power oscillator and initial sinusoidal forcing frequency of 20 Hz and voltage of 0.1 V is set throughpower oscillator. The vibration data is saved in the form of exciting force and resultant acceleration versus time. Thisprocedure is repeated for all the three test materials. From the time domain data, the graph between acceleration versustime and the force magnitude versus time is plotted and superimposed. The schematic of plot is shown in fig. 4 and thephase lag is calculated using following equation (2): (Eq. 2)Where T is time period of one cycle and t is time lag in seconds between exciting force and its response. 36
4.
F.E. Analysis and Experimental Investigation of Effect of Reinforcement Dimensions COMPOSITE ACCELEROMETER AND FORCE TRANSDUCER SPECIMEN DATA ACQUISITION FFT CLAMP EXCITER SYSTEM ANALYZER Figure 3: Experimental setup for studying damping behavior F ---- X Figure 4: Schematic of excitation force and its response3.3 Phase Lag Phase lag angle is a time by which the response lags behind the exciting force. It is a measure of the damping duringmaterial deformation. For a homogeneous material, phase lag is directly proportional to the damping, i.e. higher the phaselag angle indicates higher the material damping. Addition of reinforced glass fibers to the base polypropylene increasesthe phase lag between the exciting force and the corresponding material response. This behavior is due to the presence offiber matrix interface. IV. RESULT AND DISCUSSION4.1 Finite Element Analysis Result F.E analysis results indicate that maximum stress occurs at the sharp interface (ref. fig. 5) due to stress concentrationwhich is favorable site for cracks to appear. The stress decreases along length interface as distance increases from sharpedge as shown in fig. 5. Increased in volume fraction of fiber shows lower interfacial stress which reduces the chances ofcracking and composites shows more strength. Similar results are shown by multi fiber composites because of increasedinterface area; the stress reduces at particular volume fraction than single long fiber model. Comparisons of stresses forboth models are shown in fig. 6. Figure 5: Tensile stress nodal solutions for both long and short fiber models 37
5.
F.E. Analysis and Experimental Investigation of Effect of Reinforcement Dimensions Figure 6: Tensile stress for both long single and double fiber model at 20% and 40% volume fraction4.2 Damping Behavior The phase lag obtained from the vibration experiment for all the considered test specimen is shown in fig.7 (a-c).Due to material damping behavior, there is a lag between the excited force and its response in a time scale. Usingequation 2, the magnitude of phase lag is obtained. Fig. 8 shows the mean phase lag of all the considered test specimens.Phase lag of unreinforced, long fiber reinforced and short fiber reinforced polypropylene composites obtained fromresults are 27.61º, 28.24º and 28.36º respectively. Fig. 7: Phase lag plot between excited force and its response for (a) unreinforced (b) long fiber reinforced and (c) short fiber reinforced composite 38
6.
F.E. Analysis and Experimental Investigation of Effect of Reinforcement Dimensions Figure 8: Phase lag between excited force and its response of the test specimens4.3 Conclusion Presence of reinforced fibers in the thermoplastic material increases the strength of composite and increase involume fraction of reinforcement increases the overall strength. Reinforcement alters the damping mechanism andimproves the damping behavior. Fiber dimensions in the reinforced thermoplastic material significantly contribute to thefiber matrix interface. Short fiber reinforced material shows superior damping than long fiber reinforced material due toits more density of fiber ends for the same volume fraction. This superior damping of short fibers supports the result ofF.E. analysis of greater interfacial strength shown by short fibers composite in comparison to long fiber composite model. REFERENCES[1]. Sun C. T., Chaturvedi S. K., Gibson R. F.: Internal damping of short-fiber reinforced polymer matrix composites, Computers & Structures, 20, 391-400 (1985). DOI: 10.1016/0045-7949(85)90088-4[2]. Shive K. C., Guang Yau Tzeng,: Micromechanical modeling of material damping in discontinuous fiber three-phase polymer composites, Composites Engineering , 1, 49-60 (1991). DOI: 10.1016/0961-9526(91)90025-N[3]. Ioana C. F., Gary. G. T., Ronald F.G,: Modeling and characterization of damping in carbon nanofiber/polypropylene composites, Composites Science and Technology, 63 , 1629-1635 (2003). DOI: 10.1016/S0266-3538(03)00054-X[4]. Subramanian C., Senthilvelan S.: Development and preliminary performance evaluation of discontinuous fiber reinforced thermoplastic leaf spring, Journal of Materials: Design and Applications, 223, 3 131-142 (2009). DOI: 10.1243/14644207JMDA272[5]. Chandra R., Singh S. P., Gupta K.: Damping studies in fiber-reinforced composites, Composite Structures, 46, 41-51 (1999). DOI: 10.1016/S0263-8223(99)00041-0[6]. Gibson R.F., Hwang S.J., Kwak H.: Micromechanical modelling of damping in composites including interphase effects, Proceedings of 36th International SAMPE Symposium, Society for the Advancement of Material and Process Engineering, Covina, 1, 592-606 (1991).[7]. Lavernia E. J., Perez R. J., Zhang J.: Damping behavior of discontinuously reinforced ai alloy metal-matrix composites, Metallurgical and Materials Transactions A , 26, 2803-2818 (1995). DOI: 10.1007/BF02669639[8]. Amit Kumar Haldar, Ishan Aggarwal, Batra N. K.: Damping behavior of Discontinuous Fiber Reinforced Thermoplastic Composites. in ‘International Conference on Methods and Models in Science and Technology (ICM2ST‐10) , Chandigarh, India, 1324, 457-462 (2010). DOI: 10.1063/1.3526258[9]. Thomas Gmür, Joël Cugnoni and Alain Schorderet, A PSDT shell finite element formulation including structural damping, Computers and Structures, 88, 902-908 (2010). DOI: 10.1016/j.compstruc.2010.04.008[10]. Hassan A., Hornsby P. R., Folkes M. J.: Structure–property relationship of injection-molded carbon fiber- reinforced polyamide, composites, the effect of compounding routes, Polymer Testing, 22, 185-189 (2003). DOI: 10.1016/S0142-9418(02)00068-5[11]. Lee I., Kim B.N., Koo K.N.: Dynamic characteristics of thermoplastic composite laminates, Composites, 25, 281-286 (1994). DOI: 10.1016/0010-4361(94)90220-8[12]. Houshyar S., Shanks R. A. , Hodzic A.: Modelling of polypropylene fibre-matrix composites using finite element analysis, Express Polymer Letters, 3, No. 1, 2-12 (2009). DOI: 10.3144/expresspolymlett.2009.2[13]. Ghassemieh E., Nassehi V.: Stiffness analysis of polymeric composites using the finite element method, Advances in Polymer Technology, 20, 42-57 (2001). DOI: 10.1002/1098-2329(200121)20:1 39
Be the first to comment